#------------------------------------------------------------------------------
#$Date: 2016-02-13 14:50:18 +0200 (Sat, 13 Feb 2016) $
#$Revision: 176428 $
#$URL: svn://www.crystallography.net/cod/cif/1/52/00/1520091.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1520091
loop_
_publ_author_name
'Chen, Lijuan'
'Zhang, Fang'
'Ma, Xing'
'Luo, Jie'
'Zhao, Junwei'
_publ_section_title
;
 Two types of novel tetra-iron substituted sandwich-type arsenotungastates
 with supporting lanthanide pendants.
;
_journal_issue                   28
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              12598
_journal_page_last               12612
_journal_paper_doi               10.1039/c5dt00696a
_journal_volume                  44
_journal_year                    2015
_chemical_formula_sum            'C8 H106 As2 Fe4 La2 N2 O116 W18'
_chemical_formula_weight         6047.31
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-05-18 deposited with the CCDC.
2015-05-27 downloaded from the CCDC.
;
_cell_angle_alpha                107.303(2)
_cell_angle_beta                 99.720(2)
_cell_angle_gamma                96.736(2)
_cell_formula_units_Z            1
_cell_length_a                   12.6669(13)
_cell_length_b                   13.5788(13)
_cell_length_c                   16.3488(17)
_cell_measurement_reflns_used    8975
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      25.00
_cell_measurement_theta_min      1.72
_cell_volume                     2604.0(5)
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_collection       'Bruker XSCANS'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      296(2)
_diffrn_detector_area_resol_mean none
_diffrn_measured_fraction_theta_full 0.979
_diffrn_measured_fraction_theta_max 0.979
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0413
_diffrn_reflns_av_sigmaI/netI    0.0734
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            13131
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.72
_diffrn_standards_decay_%        none
_diffrn_standards_interval_count none
_diffrn_standards_interval_time  none
_diffrn_standards_number         none
_exptl_absorpt_coefficient_mu    21.889
_exptl_absorpt_correction_T_max  0.1275
_exptl_absorpt_correction_T_min  0.0338
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            'Light yellow'
_exptl_crystal_density_diffrn    3.856
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       flaky
_exptl_crystal_F_000             2712
_exptl_crystal_size_max          0.48
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.16
_refine_diff_density_max         2.138
_refine_diff_density_min         -3.669
_refine_diff_density_rms         0.395
_refine_ls_extinction_coef       0.00013(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.005
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     656
_refine_ls_number_reflns         8975
_refine_ls_number_restraints     24
_refine_ls_restrained_S_all      1.004
_refine_ls_R_factor_all          0.0563
_refine_ls_R_factor_gt           0.0483
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0458P)²+90.6685P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1196
_refine_ls_wR_factor_ref         0.1238
_reflns_number_gt                7806
_reflns_number_total             8975
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5dt00696a3.cif
_cod_data_source_block           5-La
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 3271 2015-04-21 07:52:19Z andrius 

 Adding full bibliography for 1520091--1520099.cif.
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               1520091
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.21390(5) 0.31251(5) 0.59641(4) 0.01528(16) Uani 1 1 d . . .
W2 W 0.46806(5) 0.44225(5) 0.68197(4) 0.01462(16) Uani 1 1 d . . .
W3 W 0.24718(5) 0.57503(5) 0.75650(4) 0.01451(15) Uani 1 1 d . . .
W4 W 0.35739(5) 0.61359(4) 0.97184(4) 0.01156(15) Uani 1 1 d . . .
W5 W 0.09591(5) 0.48747(5) 0.87935(4) 0.01365(15) Uani 1 1 d . . .
W6 W 0.15194(5) 0.25793(5) 0.94385(4) 0.01505(16) Uani 1 1 d . . .
W7 W 0.24894(5) 0.09157(5) 0.79072(4) 0.01605(16) Uani 1 1 d . . .
W8 W 0.41480(5) 0.18502(5) 0.65472(4) 0.01700(16) Uani 1 1 d . . .
W9 W 0.04523(5) 0.21530(5) 0.73193(4) 0.01427(15) Uani 1 1 d . . .
La1 La 0.11705(9) 0.23244(9) 0.32727(7) 0.0333(3) Uani 1 1 d . . .
As1 As 0.34053(11) 0.36009(11) 0.83625(10) 0.0101(3) Uani 1 1 d . . .
Fe1 Fe 0.38168(16) 0.43051(16) 1.09895(14) 0.0133(4) Uani 1 1 d . . .
O1W O 0.2406(8) 0.4520(9) 1.1540(8) 0.025(3) Uani 1 1 d . . .
O2W O 0.4112(10) 0.3178(9) 1.1622(8) 0.031(3) Uani 1 1 d . . .
O3W O 0.5530(12) 0.0482(10) 0.9289(10) 0.046(4) Uani 1 1 d . . .
O4W O 0.6891(10) 0.1180(11) 0.8248(11) 0.047(4) Uani 1 1 d . . .
O5W O 0.2614(16) 0.1386(15) 0.3793(16) 0.094(8) Uani 1 1 d . . .
O6W O 0.2836(14) 0.3752(14) 0.4062(10) 0.066(5) Uani 1 1 d . . .
O7W O -0.062(3) 0.182(2) 0.216(2) 0.089(9) Uiso 0.70 1 d P . .
O7M O -0.078(4) 0.215(4) 0.330(4) 0.051(13) Uiso 0.30 1 d P . .
O8W O 0.077(2) 0.045(2) 0.210(2) 0.132(10) Uiso 1 1 d . . .
O9W O 0.2474(19) 0.2230(17) 0.2256(12) 0.089(7) Uani 1 1 d . . .
O10W O 0.094(3) 0.359(3) 0.239(2) 0.099(10) Uiso 0.70 1 d P . .
O10M O 0.045(4) 0.301(4) 0.198(3) 0.034(10) Uiso 0.30 1 d P . .
O11W O 0.046(2) 0.078(2) 0.3738(19) 0.060(7) Uiso 0.60 1 d P . .
O11M O -0.012(3) 0.112(3) 0.378(2) 0.036(8) Uiso 0.40 1 d P . .
O12W O 0.048(3) 0.406(3) 0.381(2) 0.088(10) Uiso 0.60 1 d P . .
O12M O -0.018(3) 0.348(3) 0.388(2) 0.044(9) Uiso 0.40 1 d P . .
O13W O 0.111(2) -0.207(2) 0.9409(17) 0.106(8) Uiso 1 1 d . . .
O14W O 0.197(4) 0.012(4) 1.065(3) 0.091(13) Uiso 0.50 1 d P . .
O15W O 0.071(4) 0.531(4) 0.502(3) 0.102(15) Uiso 0.50 1 d P . .
O16W O 0.303(3) -0.064(3) 0.361(3) 0.089(11) Uiso 0.60 1 d P . .
O16M O 0.318(4) -0.121(4) 0.419(3) 0.077(14) Uiso 0.40 1 d P . .
O17W O 0.3788(17) 0.1313(12) 1.0379(10) 0.068(6) Uani 1 1 d . . .
O18W O 0.367(2) -0.120(2) 0.8982(17) 0.062(7) Uiso 0.70 1 d P . .
O18M O 0.310(4) -0.123(4) 0.918(3) 0.038(11) Uiso 0.30 1 d P . .
O19W O -0.1637(10) 0.2909(11) 0.8704(10) 0.045(4) Uani 1 1 d . . .
O20W O 0.7405(17) 0.3492(14) 0.7304(13) 0.083(7) Uani 1 1 d . . .
O21W O -0.0951(17) 0.3970(15) 0.6334(13) 0.079(6) Uani 1 1 d . . .
O22W O 0.1176(16) 0.0062(16) 0.5060(13) 0.076(5) Uiso 1 1 d . . .
O23W O 0.1362(19) -0.2008(18) 0.5099(13) 0.092(7) Uani 1 1 d . . .
O1 O 0.1351(8) 0.2915(8) 0.4929(7) 0.018(2) Uani 1 1 d . . .
O2 O 0.2882(9) 0.1977(8) 0.5694(7) 0.019(2) Uani 1 1 d . . .
O3 O 0.1862(8) 0.4407(8) 0.6678(7) 0.019(2) Uani 1 1 d . . .
O4 O 0.3424(8) 0.3322(7) 0.7209(6) 0.012(2) Uani 1 1 d . . .
O5 O 0.1150(8) 0.2368(8) 0.6427(6) 0.014(2) Uani 1 1 d U . .
O6 O 0.3402(8) 0.3960(8) 0.5841(6) 0.018(2) Uani 1 1 d U . .
O7 O 0.5548(9) 0.5122(10) 0.6392(8) 0.028(3) Uani 1 1 d . . .
O8 O 0.4980(8) 0.3022(8) 0.6371(7) 0.017(2) Uani 1 1 d . . .
O9 O 0.5444(9) 0.4618(8) 0.7897(7) 0.019(2) Uani 1 1 d . . .
O10 O 0.3841(9) 0.5485(8) 0.7303(7) 0.022(2) Uani 1 1 d . . .
O11 O 0.2228(9) 0.6633(9) 0.7010(8) 0.024(3) Uani 1 1 d . . .
O12 O 0.1112(8) 0.5598(8) 0.7941(7) 0.018(2) Uani 1 1 d U . .
O13 O 0.2736(8) 0.4728(8) 0.8523(7) 0.016(2) Uani 1 1 d . . .
O14 O 0.3154(8) 0.6672(7) 0.8692(7) 0.015(2) Uani 1 1 d . . .
O15 O 0.4809(8) 0.5902(8) 0.9375(7) 0.020(2) Uani 1 1 d . . .
O16 O 0.3558(9) 0.5292(8) 1.0368(7) 0.020(2) Uani 1 1 d . . .
O17 O 0.3940(9) 0.7401(8) 1.0514(7) 0.019(2) Uani 1 1 d . . .
O18 O 0.1929(8) 0.5990(8) 0.9637(7) 0.016(2) Uani 1 1 d . . .
O19 O -0.0274(9) 0.5184(8) 0.8990(8) 0.023(3) Uani 1 1 d . . .
O20 O 0.0476(9) 0.3623(8) 0.7763(7) 0.020(2) Uani 1 1 d . . .
O21 O 0.1217(8) 0.3949(8) 0.9443(6) 0.016(2) Uani 1 1 d . . .
O22 O 0.2235(8) 0.2616(7) 0.8206(7) 0.013(2) Uani 1 1 d . . .
O23 O 0.2884(8) 0.3144(8) 1.0032(7) 0.018(2) Uani 1 1 d . . .
O24 O 0.0871(9) 0.2402(8) 1.0237(7) 0.022(2) Uani 1 1 d . . .
O25 O 0.0232(9) 0.2105(8) 0.8433(8) 0.021(2) Uani 1 1 d . . .
O26 O 0.1822(8) 0.1209(8) 0.8932(7) 0.018(2) Uani 1 1 d . . .
O27 O 0.2366(9) -0.0442(8) 0.7679(7) 0.022(2) Uani 1 1 d . . .
O28 O 0.1025(8) 0.0885(8) 0.7199(7) 0.020(2) Uani 1 1 d . . .
O29 O 0.3849(9) 0.1417(8) 0.8614(7) 0.023(3) Uani 1 1 d . . .
O30 O 0.3055(9) 0.1077(8) 0.6941(7) 0.018(2) Uani 1 1 d . . .
O31 O 0.4567(10) 0.0819(9) 0.5835(8) 0.031(3) Uani 1 1 d . . .
O32 O 0.5062(9) 0.2068(9) 0.7596(7) 0.023(2) Uani 1 1 d . . .
O33 O -0.0849(9) 0.1675(9) 0.6712(8) 0.024(3) Uani 1 1 d . . .
O34 O 0.4832(10) -0.0050(9) 0.7473(9) 0.034(3) Uani 1 1 d D . .
Fe2 Fe 0.53368(18) 0.13618(16) 0.84558(15) 0.0174(5) Uani 1 1 d . . .
O35 O 0.615(2) -0.043(2) 0.685(2) 0.054(8) Uiso 0.50 1 d PD A 1
O36 O 0.501(3) -0.273(3) 0.668(2) 0.081(8) Uiso 0.50 1 d PD B 1
H36 H 0.5235 -0.3288 0.6553 0.122 Uiso 0.50 1 d PR B 1
N1 N 0.325(2) -0.155(3) 0.628(2) 0.044(6) Uiso 0.50 1 d PD A 1
H1A H 0.2888 -0.2077 0.5811 0.053 Uiso 0.50 1 d PR A 1
H1B H 0.3171 -0.1712 0.6764 0.053 Uiso 0.50 1 d PR A 1
H1C H 0.2996 -0.0969 0.6294 0.053 Uiso 0.50 1 d PR A 1
C1 C 0.521(3) -0.058(3) 0.695(2) 0.038(9) Uiso 0.50 1 d PD A 1
C2 C 0.444(3) -0.144(2) 0.617(2) 0.036(7) Uiso 0.50 1 d PD A 1
H2 H 0.4458 -0.1245 0.5639 0.043 Uiso 0.50 1 calc PR A 1
C3 C 0.460(2) -0.2574(18) 0.5974(15) 0.057(7) Uani 1 1 d D . .
C4 C 0.385(3) -0.344(2) 0.537(2) 0.089(10) Uani 1 1 d . B .
H4A H 0.3565 -0.3281 0.4851 0.133 Uiso 1 1 d R . .
H4B H 0.4210 -0.4034 0.5213 0.133 Uiso 1 1 d R . .
H4C H 0.3267 -0.3603 0.5640 0.133 Uiso 1 1 d R . .
O35' O 0.546(3) -0.130(3) 0.773(2) 0.068(10) Uiso 0.50 1 d PD A 2
O36' O 0.516(3) -0.212(3) 0.555(3) 0.081(8) Uiso 0.50 1 d PD B 2
H36' H 0.5008 -0.1567 0.5510 0.122 Uiso 0.50 1 d PR B 2
N1' N 0.345(3) -0.113(3) 0.599(2) 0.044(6) Uiso 0.50 1 d PD A 2
H1'A H 0.2952 -0.1560 0.5537 0.066 Uiso 0.50 1 d PR A 2
H1'B H 0.3139 -0.0655 0.6324 0.066 Uiso 0.50 1 d PR A 2
H1'C H 0.3954 -0.0799 0.5792 0.066 Uiso 0.50 1 d PR A 2
C1' C 0.484(3) -0.093(2) 0.729(2) 0.028(8) Uiso 0.50 1 d PD A 2
C2' C 0.403(3) -0.176(3) 0.651(2) 0.036(7) Uiso 0.50 1 d PD A 2
H2' H 0.3485 -0.2120 0.6737 0.043 Uiso 0.50 1 calc PR A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
As As 0.0499 2.0058 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
La La -0.2871 2.4523 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 W1 O2 99.2(5) . .
O1 W1 O3 105.1(5) . .
O2 W1 O3 155.2(4) . .
O1 W1 O5 100.0(5) . .
O2 W1 O5 90.4(4) . .
O3 W1 O5 90.0(4) . .
O1 W1 O6 97.2(5) . .
O2 W1 O6 86.8(5) . .
O3 W1 O6 85.6(4) . .
O5 W1 O6 162.8(4) . .
O1 W1 O4 169.9(4) . .
O2 W1 O4 73.2(4) . .
O3 W1 O4 82.1(4) . .
O5 W1 O4 86.8(4) . .
O6 W1 O4 76.1(4) . .
O7 W2 O9 103.3(5) . .
O7 W2 O8 101.8(5) . .
O9 W2 O8 92.7(4) . .
O7 W2 O10 100.4(5) . .
O9 W2 O10 90.3(5) . .
O8 W2 O10 156.3(4) . .
O7 W2 O6 99.6(5) . .
O9 W2 O6 156.9(5) . .
O8 W2 O6 85.8(4) . .
O10 W2 O6 82.3(5) . .
O7 W2 O4 172.4(5) . .
O9 W2 O4 83.1(4) . .
O8 W2 O4 73.6(4) . .
O10 W2 O4 83.4(4) . .
O6 W2 O4 74.3(4) . .
O11 W3 O14 100.7(5) . .
O11 W3 O10 99.4(5) . .
O14 W3 O10 91.3(5) . .
O11 W3 O12 99.4(5) . .
O14 W3 O12 90.2(5) . .
O10 W3 O12 160.6(4) . .
O11 W3 O3 103.1(5) . .
O14 W3 O3 156.2(4) . .
O10 W3 O3 86.0(4) . .
O12 W3 O3 84.9(5) . .
O11 W3 O13 170.9(5) . .
O14 W3 O13 72.2(4) . .
O10 W3 O13 86.7(4) . .
O12 W3 O13 75.3(4) . .
O3 W3 O13 84.0(4) . .
O17 W4 O16 103.0(5) . .
O17 W4 O15 103.6(5) . .
O16 W4 O15 97.8(5) . .
O17 W4 O14 94.6(4) . .
O16 W4 O14 159.2(5) . .
O15 W4 O14 88.7(5) . .
O17 W4 O18 96.9(4) . .
O16 W4 O18 86.2(5) . .
O15 W4 O18 157.6(5) . .
O14 W4 O18 80.6(4) . .
O17 W4 O13 163.6(4) . .
O16 W4 O13 88.4(5) . .
O15 W4 O13 86.2(4) . .
O14 W4 O13 72.2(4) . .
O18 W4 O13 71.8(4) . .
O19 W5 O18 101.6(5) . .
O19 W5 O21 102.3(5) . .
O18 W5 O21 92.8(4) . .
O19 W5 O20 100.6(5) . .
O18 W5 O20 157.4(4) . .
O21 W5 O20 86.4(4) . .
O19 W5 O12 98.0(5) . .
O18 W5 O12 88.5(5) . .
O21 W5 O12 159.0(4) . .
O20 W5 O12 84.5(4) . .
O19 W5 O13 170.8(4) . .
O18 W5 O13 72.5(4) . .
O21 W5 O13 85.2(4) . .
O20 W5 O13 84.9(4) . .
O12 W5 O13 75.2(4) . .
O24 W6 O23 103.0(5) . .
O24 W6 O26 101.4(5) . .
O23 W6 O26 95.4(5) . .
O24 W6 O21 100.3(5) . .
O23 W6 O21 90.8(5) . .
O26 W6 O21 155.4(4) . .
O24 W6 O25 98.3(5) . .
O23 W6 O25 158.4(5) . .
O26 W6 O25 83.7(4) . .
O21 W6 O25 81.9(4) . .
O24 W6 O22 172.0(4) . .
O23 W6 O22 84.0(4) . .
O26 W6 O22 73.6(4) . .
O21 W6 O22 83.5(4) . .
O25 W6 O22 75.0(4) . .
O27 W7 O29 103.0(5) . .
O27 W7 O30 100.5(5) . .
O29 W7 O30 89.7(5) . .
O27 W7 O26 97.5(5) . .
O29 W7 O26 91.0(5) . .
O30 W7 O26 161.4(4) . .
O27 W7 O28 96.4(5) . .
O29 W7 O28 160.6(5) . .
O30 W7 O28 86.3(5) . .
O26 W7 O28 86.9(5) . .
O27 W7 O22 166.8(4) . .
O29 W7 O22 87.7(4) . .
O30 W7 O22 87.0(4) . .
O26 W7 O22 74.4(4) . .
O28 W7 O22 73.1(4) . .
O31 W8 O32 103.4(5) . .
O31 W8 O8 100.3(5) . .
O32 W8 O8 91.5(5) . .
O31 W8 O30 100.2(5) . .
O32 W8 O30 87.8(5) . .
O8 W8 O30 159.1(4) . .
O31 W8 O2 97.5(5) . .
O32 W8 O2 158.7(5) . .
O8 W8 O2 88.4(4) . .
O30 W8 O2 84.8(4) . .
O31 W8 O4 166.7(5) . .
O32 W8 O4 88.9(4) . .
O8 W8 O4 73.9(4) . .
O30 W8 O4 85.2(4) . .
O2 W8 O4 70.7(4) . .
O33 W9 O5 99.3(5) . .
O33 W9 O20 103.1(5) . .
O5 W9 O20 89.3(4) . .
O33 W9 O25 99.6(5) . .
O5 W9 O25 161.1(4) . .
O20 W9 O25 86.7(5) . .
O33 W9 O28 101.3(5) . .
O5 W9 O28 89.1(5) . .
O20 W9 O28 155.5(4) . .
O25 W9 O28 86.9(5) . .
O33 W9 O22 172.7(4) . .
O5 W9 O22 84.8(4) . .
O20 W9 O22 82.8(4) . .
O25 W9 O22 76.3(4) . .
O28 W9 O22 72.7(4) . .
O7M La1 O5W 131.3(13) . .
O7M La1 O9W 142.5(13) . .
O5W La1 O9W 74.3(8) . .
O7M La1 O7W 42.8(14) . .
O5W La1 O7W 136.5(9) . .
O9W La1 O7W 99.8(9) . .
O7M La1 O1 81.8(13) . .
O5W La1 O1 76.3(6) . .
O9W La1 O1 135.4(5) . .
O7W La1 O1 124.5(8) . .
O7M La1 O6W 134.5(13) . .
O5W La1 O6W 74.8(6) . .
O9W La1 O6W 72.0(6) . .
O7W La1 O6W 145.6(8) . .
O1 La1 O6W 68.4(4) . .
O7M La1 O11W 66.4(14) . .
O5W La1 O11W 65.3(9) . .
O9W La1 O11W 123.7(9) . .
O7W La1 O11W 85.3(10) . .
O1 La1 O11W 70.2(7) . .
O6W La1 O11W 127.6(8) . .
O7M La1 O10W 89.6(14) . .
O5W La1 O10W 138.8(10) . .
O9W La1 O10W 67.6(10) . .
O7W La1 O10W 67.2(11) . .
O1 La1 O10W 122.0(9) . .
O6W La1 O10W 79.0(9) . .
O11W La1 O10W 152.2(11) . .
O7M La1 O12W 64.8(15) . .
O5W La1 O12W 139.2(10) . .
O9W La1 O12W 117.0(10) . .
O7W La1 O12W 82.6(11) . .
O1 La1 O12W 69.2(9) . .
O6W La1 O12W 72.7(10) . .
O11W La1 O12W 119.2(11) . .
O10W La1 O12W 55.6(12) . .
O7M La1 O12M 41.0(15) . .
O5W La1 O12M 139.8(10) . .
O9W La1 O12M 139.6(10) . .
O7W La1 O12M 70.3(11) . .
O1 La1 O12M 63.7(8) . .
O6W La1 O12M 94.0(10) . .
O11W La1 O12M 95.2(11) . .
O10W La1 O12M 72.6(11) . .
O12W La1 O12M 25.5(10) . .
O7M La1 O11M 46.6(15) . .
O5W La1 O11M 84.7(9) . .
O9W La1 O11M 140.7(9) . .
O7W La1 O11M 73.3(10) . .
O1 La1 O11M 66.9(8) . .
O6W La1 O11M 134.0(8) . .
O11W La1 O11M 20.4(8) . .
O10W La1 O11M 135.5(11) . .
O12W La1 O11M 100.6(12) . .
O12M La1 O11M 75.7(11) . .
O7M La1 O8W 89.0(14) . .
O5W La1 O8W 74.8(8) . .
O9W La1 O8W 70.2(8) . .
O7W La1 O8W 63.0(10) . .
O1 La1 O8W 131.6(7) . .
O6W La1 O8W 136.5(8) . .
O11W La1 O8W 62.7(9) . .
O10W La1 O8W 105.2(11) . .
O12W La1 O8W 145.5(11) . .
O12M La1 O8W 129.1(11) . .
O11M La1 O8W 72.4(10) . .
O22 As1 O13 98.4(4) . .
O22 As1 O4 96.3(4) . .
O13 As1 O4 99.1(5) . .
O16 Fe1 O23 92.3(5) . .
O16 Fe1 O15 93.2(5) . 2_667
O23 Fe1 O15 97.0(5) . 2_667
O16 Fe1 O9 94.7(5) . 2_667
O23 Fe1 O9 167.9(5) . 2_667
O15 Fe1 O9 92.4(5) 2_667 2_667
O16 Fe1 O2W 177.6(5) . .
O23 Fe1 O2W 86.0(5) . .
O15 Fe1 O2W 85.3(5) 2_667 .
O9 Fe1 O2W 87.2(5) 2_667 .
O16 Fe1 O1W 92.4(5) . .
O23 Fe1 O1W 87.0(4) . .
O15 Fe1 O1W 173.0(5) 2_667 .
O9 Fe1 O1W 82.9(4) 2_667 .
O2W Fe1 O1W 89.3(5) . .
O12M O7M La1 73(2) . .
O10M O10W La1 84(4) . .
O10W O10M La1 75(4) . .
O11M O11W La1 81(3) . .
O11W O11M La1 78(3) . .
O12M O12W La1 78(3) . .
O12W O12M O7M 135(4) . .
O12W O12M La1 77(3) . .
O7M O12M La1 66(2) . .
W1 O1 La1 148.8(5) . .
W1 O2 W8 121.8(5) . .
W1 O3 W3 146.7(6) . .
As1 O4 W1 134.6(5) . .
As1 O4 W8 116.8(5) . .
W1 O4 W8 94.1(3) . .
As1 O4 W2 118.2(5) . .
W1 O4 W2 91.4(3) . .
W8 O4 W2 91.4(3) . .
W9 O5 W1 154.5(6) . .
W1 O6 W2 117.8(5) . .
W8 O8 W2 121.0(5) . .
W2 O9 Fe1 143.5(6) . 2_667
W3 O10 W2 146.1(6) . .
W3 O12 W5 119.9(5) . .
As1 O13 W4 114.9(5) . .
As1 O13 W5 128.7(5) . .
W4 O13 W5 93.9(4) . .
As1 O13 W3 126.8(5) . .
W4 O13 W3 94.1(4) . .
W5 O13 W3 89.5(3) . .
W3 O14 W4 121.4(5) . .
W4 O15 Fe1 178.1(6) . 2_667
W4 O16 Fe1 167.9(7) . .
W4 O17 Fe2 164.3(6) . 2_667
W5 O18 W4 121.5(5) . .
W9 O20 W5 144.8(6) . .
W5 O21 W6 147.5(6) . .
As1 O22 W7 117.5(5) . .
As1 O22 W6 118.2(5) . .
W7 O22 W6 92.3(4) . .
As1 O22 W9 134.8(5) . .
W7 O22 W9 93.7(3) . .
W6 O22 W9 90.2(3) . .
W6 O23 Fe1 145.7(6) . .
W9 O25 W6 118.0(5) . .
W6 O26 W7 119.7(5) . .
W9 O28 W7 120.3(5) . .
W7 O29 Fe2 135.4(6) . .
W7 O30 W8 146.8(6) . .
W8 O32 Fe2 138.6(6) . .
C1' O34 C1 50(2) . .
C1' O34 Fe2 144.1(19) . .
C1 O34 Fe2 136(2) . .
O32 Fe2 O29 88.4(5) . .
O32 Fe2 O17 98.6(5) . 2_667
O29 Fe2 O17 97.0(5) . 2_667
O32 Fe2 O34 89.3(5) . .
O29 Fe2 O34 91.0(5) . .
O17 Fe2 O34 168.8(5) 2_667 .
O32 Fe2 O3W 174.5(5) . .
O29 Fe2 O3W 89.7(6) . .
O17 Fe2 O3W 86.8(5) 2_667 .
O34 Fe2 O3W 85.5(6) . .
O32 Fe2 O4W 93.4(6) . .
O29 Fe2 O4W 175.7(5) . .
O17 Fe2 O4W 86.6(5) 2_667 .
O34 Fe2 O4W 85.0(5) . .
O3W Fe2 O4W 88.2(6) . .
O34 C1 O35 127(3) . .
O34 C1 C2 118(3) . .
O35 C1 C2 114(3) . .
C3 C2 N1 100(2) . .
C3 C2 C1 119(3) . .
N1 C2 C1 112(3) . .
O36 C3 O36' 124(4) . .
O36 C3 C4 114(3) . .
O36' C3 C4 109(3) . .
O36 C3 C2 110(3) . .
O36' C3 C2 70(2) . .
C4 C3 C2 125(3) . .
O36 C3 C2' 88(3) . .
O36' C3 C2' 108(3) . .
C4 C3 C2' 112(3) . .
C2 C3 C2' 38(2) . .
O34 C1' O35' 123(3) . .
O34 C1' C2' 123(3) . .
O35' C1' C2' 114(3) . .
C3 C2' N1' 114(3) . .
C3 C2' C1' 111(2) . .
N1' C2' C1' 105(3) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O1 1.737(10) .
W1 O2 1.894(10) .
W1 O3 1.894(11) .
W1 O5 1.917(10) .
W1 O6 1.925(11) .
W1 O4 2.306(10) .
W2 O7 1.734(11) .
W2 O9 1.787(11) .
W2 O8 1.932(10) .
W2 O10 1.949(11) .
W2 O6 1.967(10) .
W2 O4 2.349(10) .
W3 O11 1.731(11) .
W3 O14 1.882(10) .
W3 O10 1.905(11) .
W3 O12 1.934(11) .
W3 O3 1.935(11) .
W3 O13 2.391(11) .
W4 O17 1.772(11) .
W4 O16 1.779(10) .
W4 O15 1.781(10) .
W4 O14 2.037(10) .
W4 O18 2.047(10) .
W4 O13 2.280(10) .
W5 O19 1.721(10) .
W5 O18 1.859(10) .
W5 O21 1.894(10) .
W5 O20 1.951(11) .
W5 O12 1.951(10) .
W5 O13 2.385(10) .
W6 O24 1.715(11) .
W6 O23 1.789(10) .
W6 O26 1.911(10) .
W6 O21 1.941(10) .
W6 O25 1.999(11) .
W6 O22 2.356(10) .
W7 O27 1.751(10) .
W7 O29 1.830(11) .
W7 O30 1.900(11) .
W7 O26 1.961(10) .
W7 O28 2.002(10) .
W7 O22 2.287(9) .
W8 O31 1.735(11) .
W8 O32 1.820(11) .
W8 O8 1.925(11) .
W8 O30 1.947(11) .
W8 O2 1.999(11) .
W8 O4 2.342(9) .
W9 O33 1.714(10) .
W9 O5 1.904(10) .
W9 O20 1.905(11) .
W9 O25 1.907(11) .
W9 O28 1.915(10) .
W9 O22 2.370(10) .
La1 O7M 2.46(5) .
La1 O5W 2.521(18) .
La1 O9W 2.52(2) .
La1 O7W 2.54(3) .
La1 O1 2.547(10) .
La1 O6W 2.551(15) .
La1 O11W 2.55(3) .
La1 O10W 2.56(3) .
La1 O12W 2.57(4) .
La1 O12M 2.58(4) .
La1 O11M 2.58(3) .
La1 O8W 2.62(3) .
As1 O22 1.804(10) .
As1 O13 1.809(10) .
As1 O4 1.816(10) .
Fe1 O16 1.933(10) .
Fe1 O23 1.950(10) .
Fe1 O15 1.956(10) 2_667
Fe1 O9 1.962(11) 2_667
Fe1 O2W 2.121(12) .
Fe1 O1W 2.144(11) .
O3W Fe2 2.066(14) .
O4W Fe2 2.083(14) .
O7M O12M 1.77(6) .
O10W O10M 0.94(5) .
O11W O11M 0.91(4) .
O12W O12M 1.13(4) .
O16W O16M 1.40(6) .
O18W O18M 0.83(5) .
O9 Fe1 1.962(11) 2_667
O15 Fe1 1.956(10) 2_667
O17 Fe2 1.983(11) 2_667
O29 Fe2 1.952(11) .
O32 Fe2 1.932(11) .
O34 C1' 1.15(3) .
O34 C1 1.15(3) .
O34 Fe2 2.049(12) .
Fe2 O17 1.983(11) 2_667
O35 C1 1.22(3) .
O36 C3 1.27(3) .
N1 C2 1.54(3) .
C1 C2 1.54(4) .
C2 C3 1.53(3) .
C3 O36' 1.29(3) .
C3 C4 1.41(4) .
C3 C2' 1.53(3) .
O35' C1' 1.23(3) .
N1' C2' 1.54(3) .
C1' C2' 1.55(4) .
